1 α, ω End Group Functionalization of RAFT Polymers Based on Pentafluorophenyl Esters and Methane Thiosulfonates Dissertation zur Erlangung des Grades "Doktor der Naturwissenschaften" im Promotionsfach Chemie am Fachbereich Chemie, Pharmazie und Geowissenschaften der Johannes Gutenberg Universität Mainz Peter J. Roth geboren in Birkenfeld Mainz, 2009
3 I Die vorliegende Arbeit wurde unter der Betreuung von Dr. Patrick Theato in der Zeit von November 2006 bis Juni 2009 am Institut für Organische Chemie der Johannes Gutenberg Universität Mainz angefertigt. Dekan: Wolfgang Hofmeister 1. Berichterstatter: Patrick Theato 2. Berichterstatter: Rudolf Zentel Tag der mündlichen Prüfung:
5 III Contents Abbreviations V Introduction 1 Views and Visions 1 Designing Functional Polymers: A Motivation for End Group Chemistry 1 Interests in End Group Functionalized Polymers 3 Polymerization Techniques: From Anionic to RAFT 4 Literature Approaches to Functional End Groups in the RAFT Process 5 References 9 Scope of this work 15 Results 17 α End Group 17 ω End Group 19 Hetero Telechelic Polymers 21 Summary and Conclusions 24 Publications P1 Synthesis of Reactive Telechelic Polymers Based on Pentafluorophenyl Esters 29 P2 A Method for Obtaining Defined End Groups of Polymethacrylates Prepared by the RAFT Process during Aminolysis 41 P3 Versatile ω End Group Functionalization of RAFT Polymers Using Functional Methane Thiosulfonates 49 P4 Hetero Telechelic Dye Labeled Polymer for Nanoparticle Decoration 63 P5 Synthesis of Hetero Telechelic α, ω Bio Functionalized Polymers 71 P6 Synthesis of Hetero Telechelic α, ω Dye Functionalized Polymer by the RAFT Process and Energy Transfer between the End Groups 81 List of Publications 95 Acknowledgement 97
7 V Abbreviations AIBN ATRP AuNP CTA DEGMA DMF DTE FRET GPC HSQC IR LCST LMA MMA MTS NBD NIPA(m) NIPMA(m) NMP NMR NP OG PBS PEG PFP QD RAFT S SAM SPR T4 TCSPC THF TLC TR TTC UV vis azobisisobutyronitrile atom transfer radical polymerization gold nanoparticle chain transfer agent diethylene glycol (monomethyl ether) methacrylate dimethylformamide dithioester fluorescence (Förster) resonance energy transfer gel permeation chromatography hetero nuclear single quantum coherence infrared lower critical solution temperature lauryl methacrylate methyl methacrylate methane thiosulfonate 7 nitro 2,1,3 benzoxadiazole N isopropyl acrylamide N isopropyl methacrylamide nitroxide mediated polymerization nuclear magnetic resonance nanoparticle Oregon Green phosphate buffered saline poly(ethylene oxide) pentafluorophenyl quantum dot (semiconductor NP) reversible addition fragmentation chain transfer styrene self assembled monolayer surface plasmon resonance thyroxin time correlated single photon counting tetrahydrofuran thin layer chromatography Texas Red trithiocarbonate ultra violet and visible (light)
9 Introduction 1 Introduction Views and Visions A one word summary of the achievements of chemistry in the twentieth century could be: polymers. An everyday life has become unthinkable without synthetic commodity polymers such as polyethylene, polypropylene, nylon or polystyrene, or commonly, plastics. The ease of producing materials with tunable mechanic properties explains the broad spreading of polymeric materials throughout construction engineering, packaging industry, transportation including space travel, and many other fields of technology. While the fundamental research on many customary plastic products has already passed its zenith, nine years into the twenty first century, functional polymers are conquering research fields on alternative energy or biotechnology and pharmacy. Semiconducting polymers are being explored for the construction of efficient solar panels and light emitting displays. Polymer pharmaceutics are drugs bound to a polymer that is intended to selectively find diseased cells. Many of the modern applications and aims rely on improved synthetic techniques to produce functionalized polymers that can create interfaces between organic materials and inorganic or biological components, thus enabling the combination of the advantages from each part of science. Looking ahead, enthusiastic researchers draw visions of solar cells printed onto textiles and of hope to cure cancer based on polymers carrying functional groups and hybrid systems including functionalized polymers. With a global energy crisis approaching and the perpetual threat of new lethal diseases, pursuing such objectives seems to be the right thing to do. The possibility to investigate novel functional polymers, however, relies on synthetic methods to construct such materials. Accordingly, there is a need to explore novel synthetic techniques leading to welldefined functional polymers easier, more accurate and with a broader range of possibilities than before. It arises the question of how and where to best install functional groups into a polymer; of a polymerization procedure and a polymer architecture. Designing Functional Polymers: A Motivation for End Group Chemistry Concerning the architectural design of a functional linear polymer chain, there are two principal possibilities: (1) functional groups incorporated into monomeric units and thus located along the polymer backbone or (2) functional groups specifically positioned at the two end groups of a polymer chain. 1. Groups statistically distributed along the polymer backbone The first approach has extensively been investigated. Activated esters, such as pentafluorophenyl (PFP) esters 1 proved to be very successful candidates for reactive polymers and are easily accessible through monomers such as PFP acrylate, PFP methacrylate 2 or PFP vinyl benzoate. 3 They react with primary and secondary amines under very mild conditions to form the respective amides. In many cases, it is not de
10 2 Introduction sired to convert every monomeric unit with the same functional amine (often, a direct polymerization of the respective amide monomer could be easier), but to statistically convert the activated units with different amines. The purposes of groups thus inserted can be to provide solubility, to act as anchor groups for inorganic nanoparticles 4,5 such as quantum dots, 6 14 to target biological materials or to bear fluorescent dyes 6,7 or pharmaceutically active drugs Some of these groups are most efficient if present only in very low concentrations, such as fluorescent dyes, running the risk of quenching effects. Incorporating multiple functionalities along a polymer backbone has however several drawbacks. If different groups, such as amines, to be installed into the polymer show different reactivities toward the reactive polymer, it becomes difficult to control the exact percentage of incorporation of each group. Even if different reactivities can be ruled out or compensated, the incorporation of functional groups is statistical and the exact amount especially of diluted functionalities per polymer chain is subject to strong variations. The intramolecular distance between two functional groups is ill defined. If there is an effect of neighboring groups during the conversion of the reactive polymer, domains differing in local composition are formed and the statistical estimations about concentration or average distances between functional groups fail. Additionally, the physical properties, such as solubility, extent of swelling, conditions causing chain collapses and insolubility, relations between molecular weight and size, or glass transition temperature are ill defined for polymers consisting of different statistically distributed side residues. 2. Functionalization of both End Groups The second approach, functionalization of the end groups of a polymer and especially the incorporation of two different functionalities onto the α and the ω end groups, poses a more considerable synthetic challenge and is less examined. However, there are distinct advantages compared to the statistical incorporation of functional groups. Through end group functionalization, defined 1:1 attachments of a polymer and another molecule can be realized. As a (linear) polymer chain has exactly two end groups, quantitative conversion of each yields a very defined number of functionalities per chain. The average distance between two functional end groups is defined through the end to end distance of the polymer chain. This can either be determined through light scattering experiments or can be estimated from tabulated relations between size and molecular weight. The polymer chain itself is not modified by the end group manipulation and thus retains its solubility behavior and its physical properties. This may be exploited to externally control the end toend distance through solvent and / or temperature and thus to control the average distance between the two functional groups. Generally, α, ω hetero telechelic polymers can be applied to build up ABC structures, where A and C are arbitrary groups and B is a polymer chain that mediates solubility and has a defined end to end distance, which depends on external parameters. Because of these advantages, there is not only an academic interest in finding improved methods for an independent α, ω functionalization, but there are also application interests and research possibilities connected to α, ω functionalized polymers.
11 Introduction 3 Interests in End Group Functionalized Polymers Defined 1:1 assemblies are especially important in biotechnology, where conjugates consisting of exactly one peptide and one polymer are desired in order to improve activity and stability of proteins 18,19 or to create stimulus responsive polymer protein conjugates Hetero telechelic polymers may be applied for the synthesis of di or multiblock copolymers or as crosslinkers for polymer networks. 27 Polymers with one functional end group are used for synthesizing polymer brushes on surfaces by a grafting to technique Stimulus responsive polymeric surfaces are of great interest for applications in microfluidics. 36 If also the opposite end group bears a functionality, this group is tethered to the surface, while having a defined distance and maximum mobility. For analytical biochemistry, planar gold surfaces are of interest, enabling the detection of proteins and other analytes through surface plasmon resonance (SPR). A hetero telechelic polymer could be interesting for bio functionalization where a targeting group could be present in a small concentration on a surface that prevents non specific binding of an analyte protein. For biosensors and chip based bioassays, often multilayers of biological components are constructed, requiring building blocks with two specific binding sites It would be of considerable interest to include telechelic synthetic polymers in these constructions, exploiting the advantages of polymers, such as flexible functionalization or stimulus responsive behavior. Energy Transfer between the End Groups Apart from planar gold surfaces, also the modification of metal or semiconductor nanoparticle (NP) surfaces is of interest. Polymers are promising materials, as hybrid materials combining the solubility, processability and functionality of the polymeric shells and the unique optical and electrical properties inherent to the NP can be obtained Semiconductor NP (QD) are used as bio labels 13,44,45 and as energy donors in biological and optoelectronic research. Gold nanoparticles (AuNP) have an intense plasmon oscillation, that can accept fluorescence excitation energy through quenching As the energy transfer efficiency is highly dependent on the distance between NP and chromophore, 53,55 there is a high scientific interest in fine tuning this distance A straightforward polymer architecture would be a hetero telechelic polymer with an anchor group at one end and a fluorescent dye at the other. Because of the high distance dependence of the FRET efficiency, FRET is a very useful tool for the investigation of molecular arrangements and processes on a nanometer scale It can be quantified by several techniques such as time resolved fluorescence measurements Many mathematical models and simulations on the evaluation of such spectroscopic data for various theoretic setups have been presented The huge potential of FRET to investigate molecular architectures on a nanometer scale thus relies on the synthetic success of placing fluorescent dyes precisely at strategic locations of molecules. If a polymer chain is equipped with two fluorescent dyes capable of FRET, invaluable information on endto end distance 67,75 84 and especially the behavior of isolated polymer chains during a lower critical solution temperature (LCST) transition could become accessible. In order to obtain well defined hetero telechelic polymers, promising synthetic techniques need to be explored and, if necessary, extended.
12 4 Introduction Polymerization Techniques: From Anionic to RAFT For several decades, anionic polymerization was the most successful method for preparing heterotelechelic (vinyl based) polymers The synthesis involved a functionalized anion for initialization and the addition of an adequately modified electrophile for termination. As long as no terminating agent is added, the terminal anion stays intact ( lives ) and allows for the formation of diblock copolymers through addition of a second monomer as soon as the first has been completely consumed. Anionic polymerization is thus also termed living polymerization. However, due to the high reactivity of carbon anions, anionic polymerizations are very intolerant toward functional groups and require an absolute absence of protic solvents. Many functional end groups, including many fluorescent dyes or groups with biological uses are thus not applicable. The end of the twentieth century saw the beginning and steady rise of controlled radical polymerization. Most prominent are atom transfer radical polymerization (ATRP), 88,89 nitroxide mediated polymerization (NMP) 90 and reversible addition fragmentation chain transfer (RAFT) polymerization. 91 Compared to a free radical polymerization, termination processes such as recombination or disproportionation of two radicals are artificially suppressed. In ATRP and NMP, equilibria between a dormant and an active (radical) species reduce the concentration of radicals. In RAFT, radicals are passed on and shared between chain transfer agents. Whereas in a free radical polymerization each radical initiator gets the chance of initiating a polymer chain, in RAFT, the propagation mechanism is initiated and controlled by the chain transfer agents. As in all three methods the propagating species are radicals, less restrictions apply to the polymerization conditions and a broader range of reactions becomes available for the functionalization of polymers including the end groups. The success of RAFT polymerization in many different fields can be followed in several reviews It is probably the most promising technique for the preparation of hetero telechelic polymers Chain transfer agents (CTAs) mediating the RAFT process are usually dithioesters or trithiocarbonates with two functional groups, although also carbon based CTAs have been described. In the following, the mechanism is briefly described for a dithioester CTA. According to the denotation of Chiefari et al., 91 the two functional groups are termed leaving group R and activating group Z and fulfill specific purposes. The same steps apply to a trithiocarbonate (or xanthate); here, the first atom of the group decoded with Z would be a sulfur (or oxygen). The RAFT mechanism starts with a fragment of a radical initiator, such as a cyano propyl radical originating from AIBN, attacking the dithioester. The Z group has the purpose to stabilize the resulting carbon based radical and encourage its formation through addition of the initiator fragment. The R group is chosen to stabilize an R based radical and is often designed to resemble the monomers intended for polymerization. The following fragmentation is thus directed into expelling the R group, which starts the polymerization. The terminal radical of the propagating chain may then add onto another dithioester moiety, setting free its R group (or an already formed polymer chain) in turn, thus transferring the radical. In summary, the polymer chain is inserted between the R group and the dithioester (DTE), resulting in the structure R(α) polymer DTE Z(ω). The RAFT process thus has a great potential in producing heterotelechelic polymers. The trick is to employ suitable R and Z groups which enable installing the desired end groups either before or after polymerization, but which do not influence the polymerization mechanism.
13 Introduction 5 R S Z S I R S Z S I R S Z S I R M P m I P n P m S Z S P P m S Z S P P S Z S P M M R S S M R S S Z Z The RAFT mechanism Initiation, propagation, and equlibria providing chain transfer. I: initiator fragment, e.g. cyanopropyl radical; M: monomer; P: polymer chains. The bottom schematics show the overall reaction providing polymers with defined R and dithioester Z end groups. Literature Approaches to Functional End Groups in the RAFT Process In this chapter, methods to modify either the R or the Z group of chain transfer agents are discussed separately. Generally, a combination of two suitable methods may be employed to create a hetero telechelic polymer. 1. Modification of the R /α Group In RAFT, propagating chains are initiated by the R fragments and are thus covalently linked to the R groups by a C C bond. The modification of a CTA to include a functional or reactive R group is thus a very common and expedient way to introduce a certain α end group. Among others, CTAs with dye, 111,112 dopamine, 113 PEG, 114 poly ethylene, 115 terpyridine, 116 bipyridine, 117 poly(methyl silsesquioxane), 118 galactose, 119 biotin, 120,121 pegylated lysine 122 or C18 alkyl chain 123 R groups have been designed and employed for polymerization. Reactive N hydroxysuccinimide (NHS) ester, 119 acid, 124 azide, 26, alkynyl 126, or (protected) amine 105 α end groups have allowed polymer modifications through post polymerization reactions.
14 6 Introduction 2. Modification of the Z /ω Group The Z group is not directly attached to the polymer chain, but linked to it via the dithioester or trithiocarbonate. The modification of the Z/ω group is more challenging compared to the R/α group. Synthetic attempts toward hetero telechelic α, ω functionalized polymers thus rely on a powerful method for ω functionalization in the first place and a compatible method for the α end group. The synthesis of CTAs with a modified Z group as prospective reactive or functional ω end group can be complex and is not very common. Alternatively, several methods to replace the dithioester or trithiocarbonate with a functionality are in use. 2.1 Z Group Functionalization CTAs with C18 alkyl chain, 123,132 azide, 133 fluorescent dye, 134 triphenylamine 135 or pyridyl disulfide 23,128,136,137 Z groups have been published. Bulmus and Davis have elegantly exploited the RAFT mechanism to produce α, ω hetero telechelic polymers with two orthogonally reactive end groups (azide and pyridyl disulfide). 128 Pyridyl disulfides 138 (along with alkyl thiosulfates (Bunte salts) 139 and alkyl methanethiosulfonates (MTS)) are reagents with an electrophilic sulfur atom which undergo very selective exchange reactions with free thiols yielding unsymmetrical disulfides. Disulfides are very stable toward air, water and other nucleophiles. They may be biologically or chemically reduced, making polymers containing molecules attached via disulfide bond possible candidates for drug delivery. 143 A major drawback of functionalizing the Z group, however, is, that the dithioester or trithiocarbonate link between the ω end group and the polymer chain is not very stable. Both groups are easily decomposed in contact with radicals, 144 heat or nucleophiles, 105,145 including water at elevated ph. 146 The group of Barner Kowollik has recently shown that even storage in cyclic ethers such as THF can cause dithioester decomposition through peroxide oxidation. 147 Additionally, it may be disadvantageous to locate a fluorescent dye beyond a dithioester or trithiocarbonate, because these groups are also chromophores and may interfere with dyes through quenching or exciplex formation. 148, Removing the dithioester(dte) / trithiocarbonate (TTC) Several methods, such as thermolysis or reduction with stannanes, 105,145 to eliminate the terminal RAFTagent have been put forward. As these methods completely remove any functionality from the ω terminus, they do not play any role for the creation of α, ω hetero telechelic polymers and are only mentioned for completeness. 2.3 Replacing the DTE / TTC Addition of Thiol onto Unsaturated Bond after Aminolysis A different strategy towards ω functionalized polymers is to make use of a terminal thiol which may be released from polystyrene derivatives and poly[(meth)acrylamides] prepared by the RAFT process by aminolysis. 27, Thiol terminated polymers have not only found extensive use in producing selfassembled monolayers on metal surfaces, such as gold nanoparticles, but they are also widely used for end group conjugation. 27, Very popular is the reaction of the terminal SH group with maleimides 27,153, or acrylates 153 via Michael addition or with iodoalkanes through nucleophilic substitution. Using this approach, poly(n isopropylacrylamide) (PNIPA) with pyrene, 155,157,158 hydroxyl 153,157 or maleimide 27 end groups or poly(methyl methacrylate) (PMMA) with hydroxyl end groups 156
15 Introduction 7 have been synthesized. However, releasing a thiol by aminolysis and subsequent conjugation has several drawbacks: (i) Maleimides do not exhibit a very strong selectivity towards thiols but also undergo Michael addition of amines. 159 Thus, a two step reaction is often employed; first, a polymer with terminal SH groups is prepared by aminolysis. After purification from the excess of amine, a functional maleimide can be added in a second step. 155 (ii) The terminal thiols are prone to oxidation by oxygen. The resulting polymer polymer disulfides do not undergo conjugation reactions, which makes it mandatory to work under inert atmosphere or add reducing agents to prevent disulfide formation. (iii) Quantitative synthesis and purification of terminal thiols fails for poly[(meth)acrylates] because the initially formed SH group backbites into the penultimate monomer unit resulting in a thiolactone, 160 thus maleimide conjugation is not quantitative 156 or even impossible with poly[(meth)acrylates] Reaction with an Excess of Diazo Initiator Perrier et al. 144 presented a versatile method to recycle the chain transfer agent by reacting polymers obtained from a RAFT polymerization with an excess of AIBN or different diazo initiators. Thereby, radicals cleave the bond between the ultimate repeating unit and the sulfur atom and saturate both emerging radicals with the radical fragments from the initiator. This method also allows the introduction of functional groups, which previously need to be installed into the diazo derivative. Such groups need to be stable toward elevated temperature and radicals. It may however occur that double molecular weight products (supposably through radical radical addition of two polymer chains) are formed. 161 Although the complete removal of terminal dithioester is apparent through the loss of the typical absorbance from the polymer, some authors 121,144 do not address the end group conversion, i.e. the percentage of incorporation of the new end group. Recently, problems to obtain functionalized end groups with certain polymers by the use of diazo compounds have been reported. 145,162 The Maynard group has utilized a diazo initiator carrying a protected maleimide to replace the trithiocarbonate end group with a bio reactive functionality. 121,163 In combination with a biotin functionalized R group, hetero telechelic bio functionalized polymers could be obtained. The deprotection step of the maleimide via retro Diels Alder reaction however required harsh conditions that caused cleavages of ester bonds. 121 Poly[(meth)acrylates], such as poly[ethylene glycol methacrylates] are thus not eligible for this approach. 2.4 Diels Alder Addition of Dienes onto DTE The groups of Barner Kowollik and Stenzel have recently presented the addition of dienes onto the thiocarbonyl double bond of diethoxyphosphoryldithioformate and pyridin 2 yldithioformate end groups of polystyrene via a hetero Diels Alder reaction. The reaction yielded dithioketal cyclohexenes in very high yields and also allowed the formation of 2, 3 and 4 arm stars
16 8 Introduction 3. Summary Incorporation of functional or reactive groups, which do not interfere during polymerization, into the R group of a CTA is a common and expedient method for modification of the α end group. A modified Z group may be retained as ω end group, but will be connected to the polymer chain via a very labile link. Terminal thiols, which may be released by aminolysis, undergo side reaction on poly[(meth)acrylates], circumventing a reaction with a maleimide or similar reagent. Side products may also be formed during exchange of the terminal RAFT agent with a modified diazo compound. End groups installed by this method need to survive heat and radicals and may need harsh conditions for deprotection, thus excluding poly[(meth)acrylates] from eligible polymers. In order to find a versatile synthetic access to stable, highly functionalized hetero telechelic polymers including poly[(meth)acrylates], there is the need of developing improved methods for the modification of terminal dithioesters.
17 References 9 References  Theato, P. J. Polym. Sci. A 2008, 46,  Eberhardt, M.; Theato, P. Macromol. Rapid Commun. 2005, 26,  Nilles, K.; Theato, P.Europ. Polym. J. 2007, 43,  M. Zorn, S. Meuer, N. M. Tahir, Y. Khalavka, C. Sönnichsen, W. Tremel, R. Zentel J. Mater. Chem., 2008, 18,  M. Zorn, R. Zentel Macromol. Rapid Commun., 2008, 29,  Potapova, I., Mruk, R.; Prehl, S.; Zentel, R.; Basché, T.; Mews, A. J. Am. Chem. Soc. 2003, 125,  Potapova, I., Mruk, R.; Hübner, C.; Zentel, R.; Basché, T.; Mews, A. Angew. Chem. Int. Ed. 2005, 44,  Tahir, M. N.; Eberhardt, M.; Theato, P.; Faiß, S.; Janshoff, A.; Gorelik, T.; Kolb, U.; Tremel, W. Angew. Chem. 2006, 118,  Muhammad Nawaz Tahir, M.N.; Zink, N.; Eberhardt, M.; Therese, H. A.; Ute Kolb, Theato, P.; Tremel, W. Angew. Chem. 2006, 118,  Meuer, S.; Braun, L.; Zentel, R. Chem. Commun  X. Lou, R. Daussin, S. Cuenot, A. S. Duwez, C. Pagnoulle, C. Detrembleur, C. Bailly and R. Jerome, Chem. Mater., 2004, 16,  X. Zhao, X. Ding, Z. Zheng, Y. Peng, C. Tian, J. Wang, X. Long Huaxue Jinzhan 2005, 17,  A.F.E. Hezinger, J. Teßmar, A. Göpferich Eur. J. Pharm. Biopharm. 2008, 68,  M. T. Fernández Argüelles, A. Yakovlev, R. A. Sperling, C. Luccardini, S. Gaillard, A. Sanz Medel, J. M. Mallet, J. C. Brochon, A. Feltz, M. Oheim, W. J. Parak Nano Lett., 2007, 7,  H. Ringsdorf, J. Polym. Sci. Polym. Symp. 1975, 51,  Haag, R.; Kratz, F. Angew. Chem., Int. Ed. 2006, 45,  Liu, S.; Maheshwari, R.; Kiick, K. L. Macromolecules 2009, 42, 3 13  Caliceti, P.; Veronese, F. M.; Adv. Drug Delivery Rev. 2003, 55,  Veronese, F. M.; Biomaterials 2001, 22, 405 Lutz, J. F.; J. Polym. Sci. A 2008, 46,  Alarcón, C. d. l. H.; Pennadam, S.; Alexander, C. Chem. Soc. Rev. 2005, 34,  Gil, E. S.; Hudson, S. M. Prog. Polym. Sci. 2004,  Boyer, C.; Bulmus, V.; Liu, J.; Davis, T. P.; Stenzel, M. H.; Barner Kowollik, C J. Am. Chem. Soc. 2007,129,  Heredia, K. L.; Bontempo, D.; Ly, T.; Byers, J. T.; Halstenberg, S.; Maynard, H. D. J. Am. Chem. Soc. 2005, 127,  Shimoboji, T.; Larenas, E.; Fowler, T.; Hoffman, A. S.; Stayton, P. S. Bioconjugate Chemistry 2003, 14,  Li, M.; De, P.; Gondi, S. R.; Sumerlin, B. S. Macromol. Rapid Commun. 2008, 29,  Li, M.; De, P.; Gondi, S. R.; Sumerlin, B. S. J. Polym. Sci. A 2008, 46,  Shan, J.; Tenhu, H. Chem. Commun. 2007,  Corbierre, M. K.; Cameron, N. S.; Sutton, M.; Mochrie, S. G. J.; Lurio, L. B.; Rühm, A.; Lennox, R. B. J. Am. Chem. Soc. 2001, 123,  Corbierre, M. K.; Cameron, N. S.; Lennox, R. B. Langmuir 2004, 20,  Raula, J.; Shan, J.; Nuopponen, M.; Niskanen, A.; Jiang, H.; Kauppinen, E.; Tenhu, H. Langmuir 2003, 19,  Filali, M.; Meier, M. A. R.; Schubert, U. S.; Gohy, J. F. Langmuir 2005, 21,  Radhakrishnan, B.; Ranjan, R.; Brittain, W. J. Soft Matter 2006, 2,
18 10 References  Lyatskaya, Y.; Balazs, A. C. Macromolecules 1998, 31,  Husseman, M.; Malmström, E. E.; McNamara, M.; Mate, M.; Mecerreyes, D.; Benoit, D. G.; Hedrick, J. L.; Mansky, P.; Huang, E.; Russell, T. P.; Hawker, C. J. Macromolecules 1999, 32,  Whitesides, G. M.; Nature 2006, 442,  Homola, J.; Yee.; S. S.; Gaugitz, G.; Sens. Actuators B 1999, 54, 3 15  Homola, J. Anal. Bioanal. Chem 2003, 377,  Homola, J. Chem Rev. 2008, 108,  Spinke, J.; Liley, M.; Schmitt, F. J.; Guder, H. J.; Angermaier, J.; Knoll, W. Langmuir 1993, 9,  Sun, X. L.; Faucher, K. M.; Houston, M.; Grande, D.; Chaikof, E. L. J. Am. Chem. Soc. 2002, 124,  Ladd, J.; Boozer, C.; Yu, Q.; Chen, S.; Homola, J.; Jiang, S. Langmuir, 2004, 20,  Su, X.; Wu, Y. J.; Robolek, R.; Knoll, W. Langmuir, 2005, 21,  I. L. Medintz, H. Tetsuo, H. T. Uyeda, E. R. Goldmann, H. Mattoussi Nature Materials. 2005, 4,  M. Bruchez, M. Moronne, P. Gin, S. Weiss, A. P. Alivisatos, Science 1998, 281, 2013  A. R. Clapp, I. L. Medintz, H. Mattoussi Chem. Phys. Chem. 2006, 7,  D. M. Willard, L. L. Carillo, J. Jung, A. Van Orden, Nano Lett. 2001, 1, 469  Jesse M. Klostranec and Warren C. W. Chan Adv. Mater. 2006, 18,  W. U. Huynh, J. J. Dittmer, A. P. Alivisatos, Science 2002, 295, 2425  S. Coe,W. K.Woo,M. Bawendi, V.Bulovic, Nature 2002, 420, 800  N. Tessler, V. Medvedev, M.Kazes, S. Kan, U. Banin, Science 2002, 295, 1506  E. Dulkeith, A. C. Morteani, T. Niedereichholz, T. A. Klar, J. Feldmann, S. A. Levi, F. C. J. M. van Veggel, D. N. Reinhoudt M. Möller, D. I. Gittins Phys. Rev. Lett. 2002, 89,  Kim E. Sapsford, Lorenzo Berti, and Igor L. Medintz Angew. Chem. Int. Ed. 2006, 45,  C. S. Yun, A. Javier, T. Jennings, M. Fisher, S. Hira, S. Peterson, B. Hopkins, N. O. Reich, G. F. Strouse J. Am. Chem. Soc. 2005, 127,  J. R. Lakowicz Anal. Biochem. 2005, 337,  S. Saini, G. Srinivas, B. Bagchi J. Phys. Chem. B, 2009, 113,  E. Dulkeith, M. Ringler, T. A. Klar, J. Feldmann, A. M. Javier, W. J. Parak, Nano Lett. 2005, 5, 585  S. H. Bae, S. I. Yoo, W. K. Bae, S. Lee, J. K. Lee, B. H. Sohn Chem. Mater. 2008, 20,  G. Schneider, G. Decher, N. Nerambourg, R. Praho, M.H. V. Werts, M. Blanchard Desce Nano Lett. 2006, 6,  H. Imahori, Y. Kashiwagi, Y. Endo, T. Hanada, Y. Nishimura, I. Yamazaki, Y. Araki, O. Ito, S. Fukuzumi, Langmuir 2004, 20, 73.  Stryer, L; Haugland, R. P. Proc. Nat. Acad. Sci.USA 1967, 58,  Stryer, L. Science, 1968, 162, 526; (c) Stryer, L. Ann. Rev. Biochem. 1978, 47,  Förster, T. Ann. Phys. (N. Y.) 1948, 2, 55 57;  Förster, T. Z. Naturforsch. Teil A 1949, 4, 321;  Förster, T. Discuss. Faraday Soc. 1959, 27, 7  Scholes, G. D. Annu. Rev. Phys. Chem ,  Lakowicz, J. R. Principles of Fluorescence Spectroscopy, Kluwer Academic / Plenum, New York, 1999  Xu, Q. H.; Wang, S.; Korystov, D.; Mikhailovsky, A.; Bazan, G. C.; Moses, D.; Heeger, A. J. Proc. Nat. Acad. Sci.USA 2005, 102,  Vyprachtický, D.; Pokorná, V.; Pecka, J.; Mikeš, F. Macromolecules 1997, 30,  Grinvald, A.; Haas, E.; Steinberg, I. Z. Proc. Nat. Acad. Sci.USA 1972, 69,  Frederickson, G. H.; Andersen, H. C.; Frank, C. W. J. Chem. Phys. 1983, 79,  Roy, A. K.; Blumen, A. J. Chem. Phys. 1989, 91,  Bodunov, E, N.; Berberan Santos, M. N.; Martinho, J. M. G. J. Luminescence 2002, 96,  Farinha, J. P. S.; Martinho, J. M. G J. Chem. Phys. 2008, 112,
19 References 11  Steinberg, I. Z. Ann. Rev. Biochem. 1971, 40, ;  Haas, E.; Wilchek, M.; Katchalski Katzir, E.; Steinberg, I. Z. Proc. Nat. Acad. Sci USA 1975, 72, ;  Haas, E.; Katchalski Katzir, E.; Steinberg, I. Z. Biopolymers, 1978, 17, 11 31;  Katchalski Katzir, E.; Haas, E.; Steinberg, I. Z. Ann. N. Y. Acad. Sci. 1981,  Winnik, M. A.;, Sinclair, A. M.; Beinert, G. Can. J. Chem. 1985, 63, ;  Winnik, M. A.;, Sinclair, A. M. Macromolecues. 1985, 18,  Ni, S.; Juhué, D.; Moselhy, J.; Wang, Y.; Winnik, M. A. Macromolecules 1992, 25,  Matějíček, P.; Limpouchová, Z.; Uhlík, F.; Procházka, K.; Tuzar, Z.; Webber, S. E. Macromolecules 2002, 35, 9487;  Uhlík, F.; Limpouchová, Z.; Matějíček, P.; Procházka, K. Macromolecules 2002, 35,  Slomkowski, S.; Winnik, M. A. Macromolecules 1986, 19,  Al Takritty, E. T. B.; Jenkins, A. D:; Walton, D. R. M. Makromol. Chem 1990, 191,  Al Takritty, E. T. B.; Jenkins, A. D:; Walton, D. R. M. Makromol. Chem 1990, 191, ;  Al Takritty, E. T. B.; Jenkins, A. D:; Walton, D. R. M. Makromol. Chem 1990, 191, ;  Wang, J.; Matyjaszewski, K. J. Am. Chem. Soc. 1995, 117, ;  Matyjaszewski, K.; Xia, J. Chem. Rev. 2001, 191,  Hawker, C. J. J. Am.Chem. Soc. 1994, 116,  Chiefari, J.; Chong, Y. K.; Ercole, F.; Krstina, J.; Jeffery, J.; Le, T. P. T.; Mayadunne, R. T. A.; Meijs, G. F.; Moad, C. L.; Moad, G.; Rizzardo, E.; Thang, S. H. Macromolecules 1998, 31,  G. Moad, E. Rizzardo, S. H. Thang. Aust. J. Chem. 2005, 58,  G. Moad, E. Rizzardo, S. H. Thang. Aust. J. Chem. 2006, 59,  G. Moad, E. Rizzardo, S. H. Thang. Polymer 2008, 49,  G. Moad, E. Rizzardo, S. H. Thang. Acc. Chem. Res. 2008, 41,  E. Rizzardo, G. Moad, S. H. Thang, Reversible Addition Fragmentation Chain Transfer, in Encyclopedia of Polymer Science and Technology 2009, DOI: / pst564 (John Wiley & Sons, Inc.).  E. Rizzardo, G. Moad, S. H. Thang, in Handbook of RAFT Polymerization (Ed. C. Barner Kowollik), 2008, pp (Wiley VCH: Weinheim, Germany).  C. Barner Kowollik, Ed. Handbook of RAFT Polymerization; Wiley VCH: Weinheim, Germany,  C. Barner Kowollik, S. Perrier. J. Polym. Sci., Part A, Polym. Chem. 2008, 46,  B. Quiclet Sire, S. Z. Zard. Chemistry A European Journal 2006, 12,  M. H. Stenzel, in Handbook of RAFT Polymerization (Ed. C. Barner Kowollik), 2008, pp (Wiley VCH: Weinheim, Germany).  L. Barner, T. P. Davis, M. H. Stenzel, C. Barner Kowollik. Macromol. Rapid. Commun. 2007, 28,  C. L. McCormick, S. E. Kirkland, A. W. York. Polym. Rev. 2006, 46,  C. L. McCormick, B. S. Sumerlin, B. S. Lokitz, J. E. Stempka. Soft Matter 2008, 4,  Moad, G.; Chong, Y. K.; Postma, A.; Rizzardo, E.; Thang, S. H. Polymer 2005, L. Barner, S. Perrier, in Handbook of RAFT Polymerization (Ed. C. Barner Kowollik), 2008, pp (Wiley VCH: Weinheim, Germany).  G. Moad, C. Barner Kowollik, in Handbook of RAFT Polymerization (Ed. C. Barner Kowollik), 2008, pp (Wiley VCH, : Weinheim, Germany).  M. L. Coote, E. H. Krenske, E. I. Izgorodina, in Handbook of RAFT Polymerization (Ed. C.Barner Kowollik), 2008, pp 5 49 (Wiley VCH: Weinheim, Germany).  B. Klumperman, J. B. McLeary, E. T. A. van den Dungen, G. Pound. Macromol. Symp.2007, 248,  P. Vana. Macromol. Symp. 2007, 248,  Such, G. K.; Evans, R. A.; Davis, T. P. Macromolecules 2006, 39,  P. Geelen, B. Klumperman. Macromolecules 2007, 40,  J. Liu, W. Yang, H. M. Zareie, J. J. Gooding, T. P. Davis. Macromolecules 2009, 42,
20 12 References  A. M. dos Santos, T. Le Bris, C. Graillat, F. D Agosto, M. Lansalot. Macromolecules 2009, 42,  R. Briquel, J. Mazzolini, T. L. Bris, O. Boyron, F. Boisson, F. Delolme, F. D'Agosto, C. Boisson, R. Spitz. Angew. Chem., Int. Ed. Engl. 2008, 47,  G. C. Zhou, Harruna, II. Anal. Chem. 2007, 79,  G. Zhou, J. He, I. I. Harruna. J. Polym. Sci., Part A, Polym. Chem. 2007, 45,  Kessler, D. Inorganic Organic Hybrid Polymers: Solution Processablible Coating Materials for Defined Surface Functionalization, University of Mainz, Dissertation  Bathfied, M.; D Agosto, F.; Spitz, R.; Charreye, M. T ; Delair, T. J. Am. Chem. Soc. 2006, 128,  Hong, C. Y.; Pan, C Y. Macromolecules 2006, 39,  Heredia, K. L.; Grover, G. N.; Tao, L.; Maynard, H. D. Macromolecules, 2009, 42,  You, Y.; Oupický, D. Biomacromolecules 2007, 8,  Kujawa, P.; Tanaka, F.; Winnik, F. M. Macromolecules 2006, 39,  Nicolas, J.; Mantovani, G.; Haddleton, D. M. Macromol. Rapid. Commun. 2007, 27,  Gondi, S. R.; Vogt, A. P.; Sumerlin, B. S. Macromolecules 2007, 40,  Quémener, D.; Davis, T. P.; Barner Kowollik, C.; Stenzel, M. H. Chem. Commun. 2006,  Ladmiral, V.; Legge, T. M.; Zhao, Y.; Perrier, S. Macromolecules 2008, 41,  Boyer, C.; Liu, J., Bulmus, V.; Davis, T. P.; Barner Kowollik, C.; Stenzel, M. H. Macromolecules 2008, 41,  Nasrullah, M. J.; Vora, A.; Webster, D. C. Polym. Prepr. 2007, 48,  Ranjan, R.; Brittain, W. J. Macromolecules 2007, 40,  Ranjan, R.; Brittain, W. J. Macromol. Rapid Commun. 2007, 28,  Kujawa, P.; Watanabe, H.; Tanaka, F.; Winnik, F. M. Eur. Phys. J. E 2005, 17,  Chen, F.; Cheng, Z.; Zhu, J.; Zhang, W.; Zhu, X. Europ. Polym. J. 2008, 44,  Zhou, D.; Zhu, X.; Zhu, J.; Cheng, Z. J. Polym. Sci A 2008, 46,  Fu, Junwei, Zhang, Z.; Cheng, Z.; Zhu, J.; Zhang, W:; Zhu, X. Polym. Bull. 2008, 61,  Boyer, C.; Liu, J.; Wong, L.; Tippett, M.; Bulmus, V.; Davis, T. P. J. Polym. Sci A 2008, 46,  Liu, J.; Bulmus, V., Barner Kowollik, C.; Stenzel, M. H.; Davis, T. P. Macromol. Rapid Commun. 2007, 28,  Murthy, N.; Campbell, J.; Fausto, N.; Hoffman, A. S.; Stayton, P. S. Bioconjugate Chem., 2003, 14,  Milligan, B.; Swan, J. M. J. Chem. Soc. 1963,  Akabas, M. H.; Stauffer, D. A.; Xu, M.; Karlin, A. Science 1992,258,  Ramirez Latorre, J.; Yu, C. R.; Qu,X.; Perin, F.; Karlin, A.; Role, L. Nature (London) 1996, 380,  Chen, J. G.; Liu Chen, S. G.; Rudnick, G. Biochemistry 1997, 36,  Bulmus, V.; Woodward, M.; Lin, L.; Murthy, N.; Stayton, P.; Hoffman, A. S. Journal of Controlled Release 2003, 93,  Perrier, S.; Takolpuckdee, P.; Mars, C. A. Macromolecules 2005, 38,  Postma, A.; Davis, T. P.; Evans, R. A.; Li, G.; Moad, G.; O Shea,M. S. Macromolecules 2006, 39,  Thomas, D. B.; Convertine, A. J.; Hester, R. D.; Lowe, A. B.; McCormick, C. L. Macromolecules 2004, 37,  Gruendling, T.; Pickford, R.; Guilhaus, M.; Barner Kowollik, C. J. Polym. Sci A 2008, 46,  Farinha, J. P. S.; Relógio, P.; Charreyre, M. T.; Prazeres, T. J. V.; Martinho, J. M. G. Macromolecules 2007, 40,  Kitchin, A. D.; Velate, S.; Chen, M.; Ghiggino, K. P.; Smith, T. A.; Steer, R. P. Photochem. Photobiol. Sci 2007, 6,  Lowe, A. B.; Sumerlin, B. S.; Donovan, M. S.; McCormick, C. L. J. Am. Chem. Soc. 2002, 124,  Zhu, M. Q.; Wang, L. Q.; Exarhos, G. J.; Li, A. D. Q. J. Am. Chem. Soc. 2004, 126,  Shan, J.; Nuopponen, M.; Jiang, H.; Kauppinen, E.; Tenhu, H. Macromolecules 2003, 36,
A Novel Bioconjugation Technology for Assay Development and More! Presentation overview Who we are Solutions we provide for our customers Solulink s technology Linking system The Solulink advantage Applications
CHEM CHEMISTRY Note: See beginning of Section F for abbreviations, course numbers and coding. CHEM 1041 General Chemistry I 3 ch (3C 1T) Introductory course designed primarily for B.Sc. students. Topics
Combinatorial Chemistry and solid phase synthesis seminar and laboratory course Topic 1: Principles of combinatorial chemistry 1. Introduction: Why Combinatorial Chemistry? Until recently, a common drug
EXPERIMENT 5: DIPEPTIDE RESEARCH PROJECT Pre-Lab Questions: None. 64 I. Background Information DIPEPTIDE RESEARCH PROJECT Methods developed by organic chemists for the synthesis of biopolymers have had
UNR Chemistry Courses Changes to implement the UCCSN Common Course Numbering Initiative Effective beginning with Summer 2003 term Old CHEM courses (2002-2003 catalog) 100 MOLECULES AND LIFE IN THE MODERN
Chemical Synthesis Spontaneous organization of molecules into stable, structurally well-defined aggregates at the nanometer length scale. Overview The 1-100 nm nanoscale length is in between traditional
Problem 1. (12 points total, 4 points each) The molecular weight of an unspecified protein, at physiological conditions, is 70,000 Dalton, as determined by sedimentation equilibrium measurements and by
Supporting Information DNA Assembly and Enzymatic Cutting in Solutions: A Gold Nanoparticle Based SERS Detection Strategy Elizabeth Crew 1, Hong Yan 1, Liqin Lin 1, Jun Yin 1, Zakiya Skeete 1, Timur Kotlyar
Molecular Spectroscopy UV-Vis Spectroscopy Absorption Characteristics of Some Common Chromophores UV-Vis Spectroscopy Absorption Characteristics of Aromatic Compounds UV-Vis Spectroscopy Effect of extended
Control Strategies for Synthetic Therapeutic Peptide APIs Part III: Manufacturing Process Considerations By Brian Gregg,Aleksander Swietlow,Anita Y. Szajek,Harold Rode,Michael Verlander,Ivo Eggen USP's
Peptides: Synthesis and Biological Interest Therapeutic Agents Therapeutic peptides approved by the FDA (2009-2011) 3 Proteins Biopolymers of α-amino acids. Amino acids are joined by peptide bond. They
Publications Peer-reviewed Articles 21) Doris Abt, Bernhard V.K.J. Schmidt, Ognen Pop-Georgievski, Alexander S. Quick, Denis Danilov, Nina Y. Kostina, Michael Bruns, Wolfgang Wenzel, Martin Wegener, Cesar
MODERN PERSPECTIVES ON PEPTIDE SYNTHESIS INTRODUCTION WHITEPAPER www.almacgroup.com The complexity of synthetic peptide products, whether as reagents used in research or as therapeutic APIs, is increasing.
EXAM I I. / 6 September 25, 2000 Biochemistry I II. / 26 BIH421/621 III. / 8 TOTAL /100 I. MULTIPLE HOIE (6 points) hoose the BEST answer to the question by circling the appropriate letter. 1. An amino
Reactions of Alcohols Alcohols are versatile organic compounds since they undergo a wide variety of transformations the majority of which are either oxidation or reduction type reactions. Normally: Oxidation
Pharmaceutical Nanotechnology Pharmaceutical Nanotechnology Development of Gold-Chitosan-coated PLGA Nanoparticles Marius Hittinger 28.04.2011 Supervisor: Juniorprofessor Dr. Marc Schneider Pharmaceutical
Ultraviolet Spectroscopy The wavelength of UV and visible light are substantially shorter than the wavelength of infrared radiation. The UV spectrum ranges from 100 to 400 nm. A UV-Vis spectrophotometer
Organic Chemistry Questions 1 Molecules of 1-propanol and 2-propanol have different (1) percentage compositions (2) molecular masses (3) molecular formulas (4) structural formulas 2 Which compound is an
Anisotropy Measurement Using the Agilent Cary Eclipse Fluorescence Spectrophotometer A Versatile Instrument for Accurate Measurements Technical Overview Authors Dr. Fabian Zieschang, Katherine McNamara,
Technology StrengthS T3P Propane Phosphonic Acid Anhydride The coupling agent of the future Coupling and water removal are synthesis tools that stand at the cutting edge of purity and cost effective manufacture
Surface activation of plastics by plasma for adhesion promotion Uwe Stöhr, Ph. D. 1 Introduction In many fields a good adhesion between two materials is necessary. The adhesion should exist at the whole
Carboxylic Acids When a carbonyl carbon also bears a hydroxyl group, then these compounds are appreciably acidic, and are called carboxylic acids. R Carboxylic acids are classified according to the substituent
1) Technical informations - a) How does it work? - b) Purification - c) Quality Control 2) Standard synthesis - a) Standard peptides - b) Modified peptides - c) Shipment and Delivery Time - d) How to order?
Quality Now Certified to ISO 90012008 Quality Policy It is Peptides International's goal is to achieve complete customer satisfaction by addressing customer needs and delivering what we promise. The company
Pulsed laser deposition of organic materials PhD theses Gabriella Kecskeméti Department of Optics and Quantum Electronics University of Szeged Supervisor: Dr. Béla Hopp senior research fellow Department
CHAPTER 1 INTRODUCTION 1.1 Research Background Diabetes mellitus is a disease in which the body cannot produce sufficient insulin in their pancreas to adequately control the level of glucose in their blood
Topics to be Covered Elements of Addition Polymerization Branching and Tacticity The Effect of Crystallinity on Properties Chapters 1 & 2 in CD (Polymer Science and Engineering) What Are Polyolefins? The
GPC/SEC: Analysis and Calibration For Low Molar Mass Macromolecules Daniela Held, Silvia Fugmann, and Peter Kilz, PSS Polymer Standards Service GmbH, Mainz, Germany. Macromolecules can range from several
SORTING PLASTICS FOR RECYCLING INTRODUCTION Description Students use the difference in densities of polymers and flame tests as a basis for the development of a scheme to separate plastics. Goals for This
Carbohydrates, proteins and lipids Chapter 3 MACROMOLECULES Macromolecules: polymers with molecular weights >1,000 Functional groups THE FOUR MACROMOLECULES IN LIFE Molecules in living organisms: proteins,
Biochemistry - I Prof. S. Dasgupta Department of Chemistry Indian Institute of Technology, Kharagpur Lecture-11 Enzyme Mechanisms II In the last class we studied the enzyme mechanisms of ribonuclease A
General Considerations The Strategy of Peptide Synthesis Making peptide bonds between amino acids is not difficult. The challenge is connecting amino acids in the correct sequence. andom peptide bond formation
CHEMISTRY UW-PARKSIDE 2015-17 CATALOG Greenquist 344 262-595-2326 College: Natural and Health Sciences Degree and Programs Offered: Bachelor of Science Major - Chemistry Minor - Chemistry Certificate -
Guide to Reverse Phase SpinColumns Chromatography for Sample Prep www.harvardapparatus.com Contents Introduction...2-3 Modes of Separation...4-6 Spin Column Efficiency...7-8 Fast Protein Analysis...9 Specifications...10
Introduction to Absorbance Spectroscopy A single beam spectrophotometer is comprised of a light source, a monochromator, a sample holder, and a detector. An ideal instrument has a light source that emits
Prentice Hall Chemistry (Wilbraham) 2008, National Student Edition - South Carolina Teacher s Edition High School C O R R E L A T E D T O High School C-1.1 Apply established rules for significant digits,
Questions- Proteins & Enzymes A. A peptide with 12 amino acids has the following amino acid composition: 2 Met, 1 Tyr, 1 Trp, 2 Glu, 1 Lys, 1 Arg, 1 Thr, 1 Asn, 1 Ile, 1 Cys Reaction of the intact peptide
UNIT 1: Biochemistry 1.4: Carbohydrates and Lipids pg. 29 38 Carbohydrates Function, primary energy source for the cell, can also be a structural component of cells and organisms. Carbohydrates are the
18.2 Protein Structure and Function: An Overview Protein: A large biological molecule made of many amino acids linked together through peptide bonds. Alpha-amino acid: Compound with an amino group bonded
arboxylic Acids arboxylic acids have one property that distinguishes them from most other organic compounds they re acidic. Now not as acidic as fuming sulfuric acid, but still pretty darned acidic. The
Alkynes: An Introduction to Organic Synthesis Alkynes Hydrocarbons that contain carbon-carbon triple bonds Acetylene, the simplest alkyne is produced industrially from methane and steam at high temperature
Back to Basics Fundamentals of Polymer Analysis Using Infrared & Raman Spectroscopy Molecular Spectroscopy in the Polymer Manufacturing Process Process NIR NIR Production Receiving Shipping QC R&D Routine
COURSE TITLE COURSE DESCRIPTION CH-00X CHEMISTRY EXIT INTERVIEW All graduating students are required to meet with their department chairperson/program director to finalize requirements for degree completion.
Identifying an Unknown Substance using Infrared Spectroscopy (I), arbon-13 Nuclear Magnetic esonance ( 13 NM), and Proton Nuclear Magnetic esonance ( 1 NM) Identifying an Unknown Substance using Infrared
193 Figure 5.1 Schematic representation of photochemical water splitting (artificial photosynthesis). Five fundamental components are needed: (1) an antenna for light harvesting, (2) a charge-separation
Reminder: These notes are meant to supplement, not replace, the laboratory manual. Oxidation of Cyclohexanol to Cyclohexanone History and Application: Oxidation reactions are incredibly important in the
Chapter 16 Conjugation, resonance, and dienes Conjugation relies on the partial overlap of p-orbitals on adjacent double or triple bonds. A common conjugated system involves 1,3-dienes, such as 1,3-butadiene.
Study of the Surface Morphology of Methyl 4-nitrobenzoate Template Thin-film Molecularly Imprinted Polymers Gary Kaganas Dartmouth College and Center for Nanomaterials Research at Dartmouth, Hanover NH
Aromatic compounds GE 1 BENZENE Structure Primary analysis revealed benzene had an... empirical formula of and a molecular formula of 6 6 Q.1 Draw out some suitable structures which fit the molecular formula
Amino Acids 20 common amino acids there are others found naturally but much less frequently Common structure for amino acid COOH, -NH 2, H and R functional groups all attached to the a carbon Ionization
İZMİR INSTITUTE OF TECHNOLOGY GRADUATE SCHOOL OF ENGINEERING AND SCIENCES DEPARTMENT OF CHEMISTRY CURRICULUM OF THE GRADUATE PROGRAMS M.S. in CHEMISTRY Core Courses CHEM 500 M. S. Thesis (0 1)NC CHEM 501
Total Organic Synthesis and Characterization of Graphene Nanoribbons Gang Li Seminar in Dong group 03/26/2014 Content History of Graphene Synthesis and Characterization and Properties of Graphene Conceptual
Chapter 2 - Chemical Foundations I. Introduction By weight, cells are about 70% water, about 1% ions, about 6% small organic molecules (including amino acids, sugars, nucleotides), and about 23% macromolecules.
M.Sc. in Nano Technology with specialisation in Nano Biotechnology Nanotechnology is all about designing, fabricating and controlling materials, components and machinery with dimensions on the nanoscale,
CHEM 334L Organic Chemistry Laboratory Revision 2.0 Diazo Coupling A Synthesis of Methyl Orange In this experiment the azo dye methyl orange is prepared by a electrophilic substitution with arenediazonium
DANGER: PEROXIDIZABLE CHEMICALS By Thomas K. Wray Many organic chemicals used in laboratory solutions and reagents can form potentially deadly peroxides - powerful oxidizing agents containing active oxygen
STRUCTURE AND PROPERTIES OF POLYMERS Pavel Kratochvíl Institute of Macromolecular Chemistry, Academy of Sciences of the Czech Republic, Prague, Czech Republic Keywords: Macromolecule, polymer, monomer,
PEPTIDE SYNTHESIS Dr. Rita P.-Y. Chen Institute of Biological Chemistry Academia Sinica 1 Solution phase chemistry -Time consuming: isolation and purification at each step -Low yield: can t drive reaction
i CHEMISTRY SYLLABUS, ASSESSMENT and UNIT PLANNERS GENERAL AIMS Students should be able to - apply and use knowledge and methods that are typical to chemistry - develop experimental and investigative skills,
TiO 2 : A New Kind of Water Treatment www.rsc.org/learn-chemistry Registered charity number 207890 3: A new kind of water treatment What is solar disinfection with titanium dioxide and how does it work?
52 May/June 2012 Intelligent use of Relative Response Factors in Gas Chromatography-Flame Ionisation Detection by Karen Rome and Allyson McIntyre, AstraZeneca, Macclesfield, SK10 2NA, UK Quantitative analysis
Problem Set 3 Solutions CH332 (SP 06) 1. Skoog problem 15-1 (omit terms (j), (k) and (m)). Draw diagrams as necessary. a) fluorescence Relaxation of an excited state by emission of a photon without a change
1 Peptide bond rotation We now consider an application of data mining that has yielded a result that links the quantum scale with the continnum level electrostatic field. In other cases, we have considered
Guidance for Industry for the Submission of Chemistry, Manufacturing, and Controls Information for Synthetic Peptide Substances Center for Drug Evaluation and Research (CDER) Center for Biologics Evaluation
Real-Time PCR Vs. Traditional PCR Description This tutorial will discuss the evolution of traditional PCR methods towards the use of Real-Time chemistry and instrumentation for accurate quantitation. Objectives
http://faculty.sau.edu.sa/h.alshehri Definition: Proteins are macromolecules with a backbone formed by polymerization of amino acids. Proteins carry out a number of functions in living organisms: - They
ab102884 FITC Conjugation Kit Protocol Antibody and protein modification This product is for research use only and is not intended for diagnostic use. Version 1 Last Updated 4 November 2013 Table of Contents
Electrophilic Aromatic Substitution (EAS) is a substitution reaction usually involving the benzene ring; more specifically it is a reaction in which the hydrogen atom of an aromatic ring is replaced as
A Look at Accelerated Photostability Testing for Packaged Food and Drinks By Dr. Oliver Rahäuser and Dr. Artur Schönlein Atlas Material Testing Technology GmbH Vogelsbergstr. 22, 63589 Linsengericht-Altenhaßlau,
Regulatory Considerations for Peptide Drug Products Larisa C. Wu Peptide Team OGD/CDER/FDA 2013 GPhA/FDA CMC Workshop June 5, 2013 This presentation reflects the views of the author and should not be construed
Chemical Engineering 160/260 Polymer Science and Engineering Lecture 13: Polymerization Techniques - Dispersed Systems Objectives! To outline polymerization techniques and describe approaches to reducing
Department of Chemistry College of Science Sultan Qaboos University Title : CHEM 3326 (Applied Spectroscopy) Credits : 3 Course Format : 2 lectures and 2 tutorials Course Text : Spectrometric Identification
Molecules 9, 14, 165-1613; doi:1.339/molecules144165 Article PE ACCE molecules I 142-349 www.mdpi.com/journal/molecules Preparation of Benzothiazole-ubstituted Carbosilane Dendrimers up to the 7 th Generation
Chemistry Biochemistry, Environmental Chemistry & Nuclear Chemistry, Pre-Pharmacy & Chemical Education Kyle A. Beran, Ph.D., Professor of Chemistry BS Angelo State University (1989); Ph.D. University of
Applications of Quantum Chemistry HΨ = EΨ Areas of Application Explaining observed phenomena (e.g., spectroscopy) Simulation and modeling: make predictions New techniques/devices use special quantum properties